Standard Specification for Zinc-Coated (Galvanized) Steel Bars for Concrete Reinforcement
A 29 - A 29M - 03 _QTI5LTAZFull description
ASTM A 123AFull description
SA 449 2007Descripción completa
ASTM for piping designFull description
Standard Specification for Carbon Steel Bolts, Studs, and Threaded Rod 60 000psi Tensile Strength
Especificación Normalizada para Barras de Acero de Baja Aleación Lisas y Corrugadas para Refuerzo de ConcretoDescripción completa
Norma ASTM caracterización materiales A 573.
ASTM A 123
ASTM A 312 A
Designation: A 751 – 07a
Standard Test Methods, Practices, and Terminology for
Chemical Analysis of Steel Products1 This standard is issued under the ﬁxed designation A 751; the number immediately following the designation indicates the year of srcinal adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript epsilon (e) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the Department of Defense.
These test methods, practi ces, and terminology were prepared to answer the need for a single document that would include all aspects of obtaining and reporting the chemical analysis of steel, stainless steel, and related alloys. Such subjects as deﬁnitions of terms and product (check) analysis variations (tolerances) required clariﬁcation. Requirements for sampling, meeting speciﬁed limits, and treatment of data usually were not clearly established in product speciﬁcations. It is intended that these test methods, practices, and terminology will contain all requirements for the determination of chemical composition of steel, stainless steel, or related alloys so that product speciﬁcations will need contain only special modiﬁcations and exceptions. 1. Scope*
2. Referenced Documents 2.1 ASTM Standards: 2 E 29 Practice for Using Signiﬁcant Digits in Test Data to Determine Conformance with Speciﬁcations E 30 Test Methods for Chemical Analysis of Steel, Cast Iron, Open-Hearth Iron, and Wrought Iron 3 E 50 Practices for Apparatus, Reagents, and Safety Considerations for Chemical Analy sis of Metals, Ores, and Related Materials E 59 Practice for Sampling Steel and Iron for Determination of Chemical Composition3 E 60 Practice for Anal ysis of Metals, Ores, and Related Materials by Molecular Absorption Spectrometry E 212 Test Method for Spectrographic Analysis of Carbon and Low-Alloy Steel by the Rod-To-Rod Technique 3 E 293 Test Method for Spectrographic Determination of Acid-Soluble Aluminum in Low-Alloy Steel by the Solution Technique3 E 322 Test Method for X-Ray Emission Spectrometric Analysis of Low-Alloy Steels and Cast Irons E 327 Test Method for Optical Emission Spectrometric Analysis of Stainless Type 18-8 Steels by the Point-ToPlane Technique3 E 350 Test Methods for Chemical Analysis of Carbon Steel, Low-Alloy Steel, Silicon Electrical Steel, Ingot Iron, and Wrought Iron
1.1 These test methods, practices, and terminology cover deﬁnitions, reference methods, practices, and guides relating to the chemical analysis of steel, stainless steel, and related alloys. It includes both wet chemical and instrumental techniques. 1.2 Directions are provided for handling chemical requir ements, product analyses, residual elements, and reference standards, and for the treatment and reporting of chemical analysis data. 1.3 These test methods, practices, and terminology apply only to those product standards which include these test methods, practices, and terminology, or parts thereof, as a requirement. 1.4 In cases of conﬂict, the product speciﬁcation requirements shall take precedence over the requirements of these test methods, practices, and terminology. 1.5 Attention is directed to ISO/IEC 17025 when there may be a need for information on criteria for evaluation of testing laboratories. 1.6 This standard does not purpo rt to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
1 These test methods, practices, and terminology are under the jurisdiction of ASTM Committee A01 on Steel, Stainless Steel and Related Alloys and are the direct responsibility of Subcommittee A01.13 on Mechanical and Chemical Testing and Processing Methods of Steel Products and Processes. Current edition approved June 1, 2007. Published June 2007. Originally approved in 1977. Last previous edition approved in 2007 as A 751 – 07.
2 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected] For Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website. 3 Withdrawn.
*A Summary of Changes section appears at the end of this standard.
A 751 – 07a 2.2 ISO Standards 4 ISO/IEC 17025 General Requirements for the Competence of Testing and Calibration Laboratories
E 352 Test Methods for Chemical Analysis of Tool Steels and Other Similar Medium- and High-Alloy Steels E 353 Test Methods for Chemical Analysis of Stainless, Heat-Resisting, Maraging, and Other Similar ChromiumNickel-Iron Alloys E 354 Test Methods for Chemical Analysis of HighTemperature, Electrical, Magnetic, and Other Similar Iron, Nickel, and Cobalt Alloys E 403 Method for Optical Emission Spetrometric Analysis of Carbon and Low-Alloy Steel by the Point-To-Plane Technique3 E 404 Test Method for Spectrographic Determination of Boron In Carbon and LowAlloy Steel by the Point-ToPlane Technique3 E 415 Test Method for Optical Emission Vacuum Spectrometric Analysis of Carbon and Low-Alloy Steel E 421 Test Method for Spectrographic Determination of Silicon and Aluminum in High-Purity Iron3 E 485 Test Method for Optical Emission Vacuum Spectrometric Analysis of Blast Furnace Iron by the Point-to-Plane Technique E 548 Guide for General Criteria Used for Evaluating Laboratory Competence3 E 572 Test Method for Anal ysis of Stainless and Alloy Steels by X-ray Fluorescence Spectrometry
3. Terminology 3.1 Deﬁnitions: 3.1.1 Pertaining to Analyses: 126.96.36.199 cast or heat (formerly ladle) analysis —applies to chemical analyses representative of a heat of steel as reported to the purchaser and determined by analyzing a test sample, preferably obtained during the pouring of the steel, for the elements designated in a speciﬁcation. 188.8.131.52 product, check or veriﬁcation analysis—a chemical analysis of the semiﬁnished or ﬁnished product, usually for the purpose of determining conformance to the speciﬁcation requirements. The range of the speciﬁed composition applicable to product analysis is normally greater than that applicable to heat analysis in order to take into account deviations associated with analytical reproducibility (Note 1) and the heterogeneity of the steel. NOTE 1—All of the chemical analysis procedures referenced in this document include precisio n statements with reproducibility data with the exception of Test Methods E 30.
184.108.40.206 product analysis tolerances ( Note 2 )—a permissible variation over the maximum limit or under the minimum limit
E 663 Practice for Flame Atomic Absorption Analysis3 E 743 Guide for Spectrochemical Laboratory Quality Assurance3 E 851 Practice for Evaluation of Spectrochemical laboratories3 E 882 Guide for Accountability and Quality Control in the Chemical Analysis Laboratory E 1019 Test Methods for Determination of Carbon, Sulfur, Nitrogen, and Oxygen in Steel and in Iron, Nickel, and Cobalt Alloys E 1024 Guide for Chemical Analysis of Metals and Metal Bearing Ores by Flame Atomic Absorption Spectroph otometry3 E 1063 Test Method for X-Ray Emission Spectrometric Determination of Cerium and Lanthanum in Carbon and
of a speciﬁed element and applicable only to product analyses, not cast or heat analyses.
NOTE 2—The term “analys is tolerance” is often misunderstoo d. It does not apply to cast or heat analyses determined to show conformance to speciﬁed chemical limits. It applies only to product analysi s and becomes meaningful only when the heat analysis of an element falls close to one of the speciﬁed limits. For example, stainless steel UNS 30400 limits for chromium are 18.00 to 20.00 %. A heat that the producer reported as 18.01 % chromium may be found to show 17.80 % chromium by a user performing a product analysis. If the product analysis toleranc e for such a chromium level is 0.20 %, the product analysis of 17.80 % chromium would be acceptable. A product analysis of 17.79 % would not be acceptable.
220.127.116.11 proprietary analytical method—a non-standard analytical method, not published by ASTM, utilizing reference standards traceable to the National Institute of Standards and Technology (NIST) (when availabl e) or other sources referenced in Section 10. 18.104.22.168 referee analysis—performed using ASTM methods listed in 9.1.1 and NIST reference standards or methods and reference standards agreed upon between parties. The selection of a laboratory to perform the referee analysis shall be a matter of agreement between the supplier and the purchaser. 22.214.171.124 certiﬁed reference material—a specimen of material specially prepared, analyzed, and certiﬁed for chemical content under the jurisdiction of a recognized standardizing agency or group, such as the National Institute of Standards and Technology, for use by analytical laboratories as an accurate basis for comparison. Reference samples should bear sufficient
Low-Alloy Steel E 1086 Test Method for Optical Emission Vacuum Spectrometric Analysis of Stainless Steel by Point-to-Plane Excitation Technique E 1087 Practice for Sampling Molten Steel From a Ladle Using an Immersion Sampler to Produce a Specimen for Emission Spectrochemical Analysis 3 E 1097 Guide for Direct Current Plasma Emission Spectrometry Analysis E 1184 Practice for Electrothermal (Graphite Furnace) Atomic Absorption Analysis E 1282 Guide for Specifying the Chemical Compositions and Selecting Sampling Practices and Quantitative Analysis Methods for Metals, Ores, and Related Materials E 1329 Practice for Veriﬁcation and Use of Control Charts
Available from American National Standards Institute (ANSI), 25 W. 43rd St.,
4th Floor, New York, NY 10036, http://www.ansi.org.
in Spectrochemical Analysis 2
A 751 – 07a resemblance to the material to be analyzed so that no signiﬁcant differences are required in procedures or corrections (for example, for interferences or inter-element effects). 126.96.36.199 working reference materials —reference materials used for routine analytical control and traceable to NIST standards and other recognized standards when appropriate standards are available. 3.1.2 Pertaining to Elements: 188.8.131.52 intentionally added unspeciﬁed element —an element added in controlled amounts at the option of the producer
primary heat. The heat analysis shall be obtained from one remelted ingot, or the product of one remelted ingot, from each primary melt. If this heat analysis does not meet the heat analysis requirements of the speciﬁcation, one sample from the product of each remelted ingot shall be analyzed, and the analyses shall meet the heat analysis requirements. 5.2 If the test samples taken for the heat analysi s are lost, inadequate, or not representative of the heat, a product analysis of the semiﬁnished or ﬁnished product may be used to establish the heat analysis.
to obtain desirable characteristics. 184.108.40.206 residual element —a speciﬁed or unspeciﬁed element, not intentionally added, srcinating in raw materials, refractories, or air. 220.127.116.11 speciﬁed element—an element controlled to a speciﬁed range, maximum or minimum, in accordance with the requirements of the product speciﬁcation. 18.104.22.168 trace element—a residual element that may occur in very low concentrations, generally less than 0.01 %.
5.2.1 If a product analysis is made to establish the heat analysis, the product analysis shall meet the speciﬁed limits for heat analysis and the product analysis tolerances described in Section 6 do not apply.
6. Product Analysis Requirements 6.1 For product analysis, the range of the speciﬁed chemical composition is normally greater (designated product analysis tolerances) than that applicable to heat analyses to take into account deviations associated with analytical reproducibility and the heterogeneity of the steel. If several determinations of any element in the heat are made, they may not vary both above and below the speciﬁed range. 6.2 Product analysis tolerances may not be used to determine conformance to the speciﬁed heat or cast analysis unless permitted by the individual material speciﬁcation.
4. Concerning the Speciﬁcation of Chemical Composition Requirements 4.1 It is recommended that Guide E 1282 be consulted as a guide for specifying the chemical compositions for steels. 4.2 The recommended practice for specifying chemical composition limits is to limit the number of signiﬁcant ﬁgures for each element so that the number of ﬁgures to the right of the decimal point conforms to the following: Chemical Concentration Up to 0.010 %, incl. — Over 0.010 % to — 0.10 %, incl. Over 0.10 % to 3.0 %, — incl. Over3.0% —
6.3 Product analysis tolerances, where available, are given in the individual material speciﬁcations or in the general requirement speciﬁcations.
Maximum Number of Figures to the Right of the Decimal Point 0.XXXX or may be expressed as ppm 0.XXX
7. Unspeciﬁed Elements (Note 4) 7.1 Reporting analyses of unspeciﬁed elements is permitted.
NOTE 4—All commercial metals contain small amounts of various elements in addition to those which are speciﬁed. It is neither practical nor necessary to specify limits for every unspeciﬁed element that might be present, despite the fact that the presence of many of these elements is often routinely determined by the producer.
4.3 For those cases in which the composition range spans either 0.10 % or 3.0 %, the number of ﬁgures to the right of the decimal is to be determined by that indicated by the upper limit. 4.4 Technical considerations may dictate the employment of less than the number of ﬁgures to the right of the decimal as previously recommended.
7.2 Analysis limits shall be established for speciﬁc elements rather than groups of elements such as “all others,” “ rare earths,” and “balance.” 8. Sampling 8.1 Cast or Heat Analyses : 8.1.1 Samples shall be taken, insofar as possible, during the casting of a heat, at a time which, in the producer’s judgment, best represents the composition of the cast. 8.1.2 In case the heat analysis samples or analyses are lost or inadequate, or when it is evident that the sample does not truly represent the heat, representative samples may be taken from the semiﬁnished or ﬁnished product, in which case such samples may be analyzed to satisfy the speciﬁed requirements. The analysis shall meet the speciﬁed limits for heat analysis. 8.2 Check, Product, or Veriﬁcation Analyses—Unless otherwise speciﬁed, the latest revision of Practice E 59 shall be used as a guide for sampling.
NOTE 3—The recommendations should be employed to reduce the number of signiﬁcant ﬁgure s, such as from 18.00 % to 18.0 %, but a signiﬁcant ﬁgure should never be added unless there is a technical reason for so doing.
5. Cast or Heat An alysis 5.1 The producer shall perform analyses for those elements speciﬁed in the material speciﬁcation. The results of such analyses shall conform to the requirements speciﬁed in the material speciﬁcation. 5.1.1 For multiple heats, either individual heat or cast analysis or an average heat or cast analysis shall be reported. If signiﬁcant variations in heat or cast size are involved, a weighted average heat or cast analysis, based on the relative quantity of metal in each heat or cast, shall be reported. 5.1.2 For consumable electrode remelted material, a heat is
9. Test Methods 9.1 This section lists some test methods that have been
deﬁned as all the ingots remelted by the same process from a
found acceptable for chemical analysis of steels. 3
A 751 – 07a TABLE 2 Normal Elements and Ranges for Stainless Steels Using Spark Emission Spectroscopy
9.1.1 The following ASTM wet chemical test methods have been found acceptable as referee test methods and as a base for standardizing instrumental analysis techniques: Test Methods E 30 E 350 E 352 E 353 E 354 E 1019
— — — — — —
C S N2 MN P Si Cr Ni Al Mo Cu Cb
General Description antecedent to Test Methods E 350 through E 354 the basic wet chemical procedure for steels wet chemical procedure for tool steels wet chemical procedure for stainless steels wet chemical procedure for high nickel steels determination of carbon, sulfur, nitrogen, oxygen, and hydrogen, in steel and in iron, nickel, and cobalt alloys
9.1.2 The following ASTM instrumental test methods, practices, and guides may be employed for chemical analysis of steels or may be useful as a guide in the calibration and standardization of instrumental equipment for routine sampling and analysis of steels: Standard E 50 E 60 E 212 E 293 E 322 E 327 E 403 E 404
9.2.2 Analysis of stainless steels using spark emission spectroscopy (OES). See Table 2 for normal elements and ranges for stainless steels. 9.2.3 Analy sis of solutions using an atomic absorption spectrophotometer. 9.2.4 Analysis of solutions using an inductively coupled plasma emission spectrometer. 9.2.5 Determination of carbon or sulfur, or both, by combustion (in oxygen) and measurement of CO2 or SO 2, or both, by thermal conductivity or infrared detectors.
General Description apparatus, reagents, and safety photometric and spectrophotometric work spectrographic analysis of steels (rod-to-rod technique) spectrographic analysis of acid-soluble aluminum x-ray ﬂuorescence for steels spectrometric analysis of stainless steels spectrometric analysis of steels spectrographic determination of steels for boron (point-toplane technique) vacuum spectrometric analysis of steels spectrographic determination of silicon and aluminum in high-purity iron optical emission vacuum spectrometric analysis of blast
Element Ranges % C 0.002–5.0
Element Ranges % 0.0005–0.1
9.2.6 Determination of nitrogen and oxygen by fusion (in a helium atmosphere) and measurement of N 2 by thermal conductivity and oxygen by measurement of CO by infrared or thermal conductivity detectors.
furnace iron by the point-to plane technique x-ray emission spectrometric analysis of stainless steels ﬂame atomic absorption accountability and quality control determination of carbon, sulfur, nitrogen, oxygen, and hydrogen in steel and in iron, nickel, and cobalt alloys ﬂame atomic absorption x-ray emission spectrometric determination of cerium and lathanum in carbon and low-alloy steels optical emission vacuum spectrometric analysis of stainless steel by the point-to plane excitation technique sampling direct current plasma spectroscopy graphite furnace atomic absorption selecting sampling practices and analysis methods veriﬁcation and use of control charts
Element Ranges % 0.0005 – 0.3 0.0008 – 0.02
9.2.7 Analy sis of solutions using inductively coupled plasma emission spectroscopy (ICP) or direct plasma emission spectroscopy (DCP). Normal elements and ranges for stainless steels are as follows: B Ca Mg Ce Zr Ta
9.2 The following are some of the commonly accepted techniques employed for routine chemical analysis of steels. These routine analyses are the basis for the producers’ quality control/assurance programs. Proprietary methods are permissible provided the results are equivalent to those obtained from standard methods when applicable. 9.2.1 Analysis of stainless steels using x-ray ﬂuorescen ce spectroscopy (XRF). See Table 1 for normal elements and ranges for stainless steels.
9.3 There are additio nal common techni ques often used for chemical analysis of standards for instrument analysis such as: polarographic analysis, ion exchange separations, radioactivation, and mass spectrometry. 10. Reference Materials
TABLE 1 Normal Elements and Ranges for Stainless Steels Using X-Ray Fluorescence Spectroscopy Element Ranges % MN P Si Cr Ni Al Mo
10.1 For referee analys es, reference standards of a recognized standardizing agency shall be employed with preference given to NIST standard reference materials when applicable. (NIST does not produce reference standards suitable for all elements or all alloys.5)
10.1.1 When standard reference materials for certain alloys are not available from NIST, reference materials may be produced by employing ASTM standard procedures and NIST standard reference materials to the extent that such procedures and reference standard s are available. Several independent laboratories should be used for certiﬁcation of these standards and their results statistically reviewed and merged. 10.1.2 Methods not published by ASTM such as a deﬁniti ve analytical method may be used when the method is validated by analyzing certiﬁed reference materials along with the
12.1 To determine conformance with the speciﬁcation requirements, an observed value or calculated value shall be rounded in accordance with Practice E 29 to the nearest unit in the last right-hand place of values listed in the table of chemical requirements. 12.2 In the special cas e of rounding the number “5” when no additional numbers other than “0” follow the “5”, rounding shall be done in the direction of the speciﬁcation analysis limits if following Practice E 29 would cause rejection of material.
candidate reference material. Examples of deﬁnitive analytical methods include gravimetric, coulometry, titrimetric based on normality, and mass spectrometry. 10.2 Working reference materials may be used for routine analytical control.
13. Records 13.1 In addition to the test data request ed, the test records shall contain the following information as appropriate: 13.1.1 Description of the material tested, for example, heat number, grade of material, product speciﬁcation. 13.1.2 Test method( s) or unambiguous description of the nonstandard method(s) used.
11. Signiﬁcant Numbers 11.1 Laboratories shall report each element to the same number of signiﬁcant numbers as used in the pertinent material speciﬁcations. 11.2 When a chemical determination yields a greater number of signiﬁcant numbers than is speciﬁed for an element, the result shall be rounded in accordance with Section 12.
APPENDIX (Nonmandatory Information) X1. QUALITY ASSURANCE FOR VALIDITY OF ANALYTICAL RESULTS
X1.1 The requirements embodied in Guide E 548, ISO/ IEC 17025, and E 851 provide generic requirements for production of valid chemical-analysis results.
X1.3.1 Replication of sampling and testing to improve the precision of results; X1.3.2 Use of reference materials is crucial to accurate results; X1.3.3 Instr umentation that is appropriate and properly maintained; and X1.3.4 Personnel who are properly trained, ethical chemists or technicians and who work with properly documented, current standards.
X1.2 Additional pertinent standards for impro ving the competency of chemical analysis laboratories are included in Guides E 743 and E 882. X1.3 Keys to improving vali dity of chemi cal anal ytical results are as follows:
SUMMARY OF CHANGES Committee A01 has identiﬁed the location of selected changes to this standard since the last issue (A 751 – 07) that may impact the use of this standard. (Approved June 1, 2007.) (1) Revised table in 4.2. Committee A01 has identiﬁed the location of selected changes to this standard since the last issue (A 751 – 01 (2006)) that may impact the use of this standard. (Approved April 1, 2007.) (1) Replaced referenced document for laboratory evaluation. ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected] (e-mail); or through the ASTM website (www.astm.org).